Synthesis, Structure, and Magnetic and Electrical Properties of Yb(Mn,M)xAl12‒x(M = Fe, Ru;x≤ 2.5) Phases
Fulfer, Bradford W.; McAlpin, Jacob D.; Haldolaarachchige, Neel; Young, David P.; Chan, Julia Y.; Crystal Growth & Design 13 (2013) 1543–; doi:10.1021/cg301783q

data_4507565
_publ_section_title
;
 Synthesis, Structure, and Magnetic and Electrical Properties of
 Yb(Mn,M)xAl12--x(M = Fe, Ru;x&#x2264; 2.5) Phases
;
_journal_issue                   4
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              1543
_journal_paper_doi               10.1021/cg301783q
_journal_volume                  13
_journal_year                    2013
_chemical_formula_sum            'Al9.69 Fe0.32 Mn1.99 Yb'
_chemical_formula_weight         561.68
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           129
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   12.7320(10)
_cell_length_b                   12.7320(10)
_cell_length_c                   5.1123(5)
_cell_measurement_temperature    298(2)
_cell_volume                     828.72(12)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.987
_diffrn_measured_fraction_theta_max 0.987
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0216
_diffrn_reflns_av_sigmaI/netI    0.0178
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            2982
_diffrn_reflns_theta_full        33.12
_diffrn_reflns_theta_max         33.12
_diffrn_reflns_theta_min         2.26
_exptl_absorpt_coefficient_mu    15.661
_exptl_absorpt_correction_T_max  0.5081
_exptl_absorpt_correction_T_min  0.3035
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_density_diffrn    4.502
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1016
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.816
_refine_diff_density_min         -2.270
_refine_diff_density_rms         0.269
_refine_ls_extinction_coef       0.0053(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.044
_refine_ls_matrix_type           full
_refine_ls_number_parameters     43
_refine_ls_number_reflns         881
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.043
_refine_ls_R_factor_all          0.0355
_refine_ls_R_factor_gt           0.0260
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0426P)^2^+0.6924P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0664
_refine_ls_wR_factor_ref         0.0730
_reflns_number_gt                691
_reflns_number_total             881
_reflns_threshold_expression     >2\s(I)
_cod_data_source_file            cg301783q_si_006.cif
_cod_data_source_block           bwf051
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Tetragonal' changed to 'tetragonal'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_sg_symbol_H-M      'P 4/n m m'
_cod_database_code               4507565